New Controlled Release of Construction Chemicals by Encapsulation · PDF file 2016. 3....
Embed Size (px)
Transcript of New Controlled Release of Construction Chemicals by Encapsulation · PDF file 2016. 3....
Journal of Encapsulation and Adsorption Sciences, 2016, 6, 9-21 Published Online March 2016 in SciRes. http://www.scirp.org/journal/jeas http://dx.doi.org/10.4236/jeas.2016.61002
How to cite this paper: von Daake, H., Ballweg, T. and Stephan, D. (2016) Controlled Release of Construction Chemicals by Encapsulation. Journal of Encapsulation and Adsorption Sciences, 6, 9-21. http://dx.doi.org/10.4236/jeas.2016.61002
Controlled Release of Construction Chemicals by Encapsulation Henning von Daake1, Thomas Ballweg2, Dietmar Stephan1* 1Building Materials and Construction Chemistry, Technische Universität Berlin, Berlin, Germany 2Fraunhofer-Institute for Silicate Reasearch ISC, Würzburg, Germany
Received 23 December 2015; accepted 5 March 2016; published 8 March 2016
Copyright © 2016 by authors and Scientific Research Publishing Inc. This work is licensed under the Creative Commons Attribution International License (CC BY). http://creativecommons.org/licenses/by/4.0/
Abstract Encapsulation and controlled release of active agents is a common practice to improve processing and properties of materials and final products in different industries. Today, a large variety of chemical admixtures are used in construction materials, the performance of which could be im- proved by a better dosage control. This work presents investigations on the controlled release of encapsulated construction chemicals for future applications in construction materials. The high shear mixing technology was used to produce matrix based encapsulations by agglomeration ap- plied to commercially available construction materials. The agglomeration process was varied by the use of different agitator types, the variation of the agitator speed and the application of addi- tional coating materials. The particle size distribution as well as the particle shape of the pro- duced agglomerates was analyzed by automatic image evolution and scanning electron microsco- py. The release behavior of the capsules in aqueous solutions was investigated by UV spectrosco- py. The obtained results confirmed a theoretical model for the encapsulation and release of ad- mixtures, which was derived from pharmaceutical drug release concepts and adapted to construc- tion materials. The results indicate that the matrix based encapsulation is a promising technique for future applications in the field of construction materials.
Keywords Construction Chemicals, Controlled Release, Encapsulation, High Shear Agglomeration
1. Introduction The process ability of cementitious systems is governed by the chemical and mineralogical cement composition, most notably the content and modification of tricalcium aluminate (C3A), the content of soluble sulfates and the composition of the pore solution during the early stage of the hydration. It is strongly affected by physical para-
http://www.scirp.org/journal/jeas http://dx.doi.org/10.4236/jeas.2016.61002 http://dx.doi.org/10.4236/jeas.2016.61002 http://www.scirp.org http://creativecommons.org/licenses/by/4.0/
H. von Daake et al.
meters like the particle size distribution, the specific surface area and particle-particle interactions as well as the water cement ratio (w/c). Beyond that, the construction chemical industry provides a wide range of chemical admixtures, e.g. superplasticizers, retarders and accelerators, to improve the fresh and hardened material proper- ties of construction materials. Looking at the mixing process, it is the dosing time of the chemical admixture, which has a significant impact on the fresh material properties due to the rapid hydration reaction of C3A in ce- ment after first contact with water and concurrent surface growth -. The high surface area of the first hy- dration products often result in an adsorption of chemical admixtures, which are overgrown by later hydration products with the consequence of a sharp loss in performance. With regard to the early hydration process, a de- layed release of chemical admixtures would be desirable to enhance the material properties and reduce the amount of chemical admixtures for future applications.
In the fields of pharmacy, nutrition and fertilizer, encapsulation is already a well established practice to gen- erate such controlled release behavior. In general, encapsulation systems can be divided into [email protected] par- ticles and matrix based morphologies as illustrated in Figure 1. [email protected] particles are characterized by a liq- uid or solid core of active material which is covered by a single or a multiple shell around the core. For matrix based encapsulations, the active agent is bound in a solid matrix material which is partially or completely so- luble. The drug release of the matrix type encapsulation primarily depends on the properties of the matrix ma- terial whereas for [email protected] particles several release mechanisms can be applied, e.g. by diffusion, osmotic pressure or dissolution of the membrane -. Normally, solid materials are encapsulated by coating or ag- glomeration techniques whereas liquid materials are encapsulated by an additional shell, based on different physical or chemical processes. The use of encapsulation systems for the controlled admixture delivery could improve the handling, safety, processing and performance of a wide range of construction materials which are used in civil engineering for future, e.g. dry mix mortars, self-healing agents etc. This could result in an ecolog- ical as well as economic benefit for the construction industry.
It was shown by the authors in a previous work that it is possible to produce matrix type encapsulations based on supplementary cementitious materials (SCMs) containing chemical admixtures with delayed release behavior . The obtained results confirm the theory that the production process, the resulting particle size distribution as well as the release behavior of the encapsulated admixtures is mainly influenced by a combination of the ma- terials viscosity and the mixing energy which is introduced in the mixtures during the agglomeration process. As shown in Figure 2(a), a high binder viscosity, due to a combination of low water and high superplasticizer con- tent in the mixture, combined with a low energy input during the agglomeration yields in fly ash coated super- plasticizer particles. The dissolution of these encapsulations is retarded by the time span needed for washing off the fly ash coating from the particles surface. With increasing energy input or decreasing binder viscosity during the agglomeration process, a larger proportion of the binder liquid is pressed towards the particle surface result- ing in a faster admixture release in aqueous solution as given in Figure 2(b). Nonetheless, the high shear ag- glomeration technique provides an easy and reproduceable possibility to encapsulate construction chemicals in
Figure 1. Illustration of a [email protected] particle (a) and a matrix type encapsulation (b), based on .
H. von Daake et al.
Figure 2. Encapsulation and dissolution mechanism of the agglomerates depending on the binder viscosity and/or the energy input during the agglomeration process, based on .
SCM based agglomerates with retarded release behavior. Due to the maximum mean dissolution time of the ag- glomerates of 3.6 min, the objective of this research is to retard the release behavior by particle optimization which was done by a variation of the mixing tool used, the tool speed during the agglomeration process as well as by the application of different coating materials.
2. Materials and Methods 2.1. Encapsulation and Coating The encapsulation by high shear agglomeration was carried out using a standard fly ash which is commonly used as SCM for mortar and concrete applications and a dry superplasticizer powder based on melamine sul- phonate. The particle size distributions and the median particle size d50 of both materials were determined by la-
H. von Daake et al.
ser granulometric analysis (Malvern Mastersizer 2000, UK) and are given in Figure 3(a). Before the agglomera- tion, fly ash and superplasticizer were homogenized with a combination of 80/20 wt.-% in a high shear mixer (Eirich R02, Germany) using a star agitator with an impeller speed of 500 rpm for 120 s and counter-rotating mixing pot on level 1. The water saturation point of the premixed mixtures was determined by the Puntke test , which is a common method in building technology to investigate the water demand of fines.
During the mixing process, 2500 g dry mixture were agglomerated by the addition of 260 g of tap water which was sprayed in by a hand pump within 300 s (vessel speed 1, agitator speed 76 rpm). After the water ad- dition, all mixtures were agglomerated for 600 s with a varying agitator type and tool speeds between 440 and 2083 rpm. The two used agitator types, a star and a pin agitator, are depicted in Figure 3(b) and Figure 3(c). Due to the equal agitator diameters, the tool speeds of the agitators were comparable. Following, the samples were coated in a second step by the extra addition of an ordinary Portland cement CEM I 42.5 R (5.0 to 7.5 wt.-% of the production mass) or a silane based dry hydrophobic agent powder (3.0 to 5.0 wt.-% of the produc- tion mass) and further mixi